User:Missstarsineyes/sandbox

Article Evaluation
I'm evaluating the page on Ultrasonic welding, a plastic welding method. At the top of the page is a message regarding the lack of encyclopedic tone. The majority of the sentences are short. Some of the sections read as if they were taken from presentation slides. Some of the sentences seem misplaced, especially those in the "Process" section.

The lead section is short and could use more topic links. The two images on the page do not clearly show the page's topic. The sections are unbalanced in length, with the "Applications" section being longer than the other sections combined.

The "References" section is split into "Notes" and "Bibliography" subsections. The citations appear under "Notes" with varying styles; for example, some of the sources are indicated by the first author's last name with the full citation appearing in the "Bibliography" section, while one of them is just a URL to a journal article with no proper citation. Some of the sources seem inappropriate, since they are magazine articles or self-promotional, and two source links are dead.

The Talk page shows the article is rated B-class in four WikiProjects: Engineering, Metalworking, Physics/Acoustics, and Technology. There are numerous comments about problems with the article. Several problems with suggested edits have not been changed. Some comments lack authors. There is an off-topic comment.

I made two contributions to the Talk page. I noted the off-topic comment and commented on the poor quality of the references and the inconsistent formatting in the References section.

Ultrasonic welding
The existing article needs editing, as pointed out in the article evaluation. I would improve the quality of the references, correct the tone, add more information to the Process section, and add more images.

Hot plate welding
This article currently doesn't exist. This is the process I'm most familiar with.

Laser welding
This article currently doesn't exist. I have some knowledge of photonics.

Testing of plastic welds
This article currently doesn't exist. This topic is more general since it applies to all plastic welds, regardless of the process. I could focus it on either destructive or non-destructive testing.

Instructor Comments
All the topics look good to me. Please let me know which one you picked. Thanks!

Draft for Hot plate welding
Hot plate welding, also called heated tool welding, is a thermal welding technique for joining thermoplastics. A heated tool is placed against or near the two surfaces to be joined in order to melt them. Then, the heat source is removed, and the surfaces are brought together under pressure. Hot plate welding has relatively long cycle times, ranging from 10 seconds to minutes, compared to vibration or ultrasonic welding. However, its simplicity and ability to produce strong joints in almost all thermoplastics make it widely used in mass production and for large structures, like large-diameter plastic pipes.

History
Hot plate welding was first used in the early 1930s for joining PVC. It gained in popularity with the prevalence of polyolefins, which are difficult to adhesively bond. By the 1960s, it was among the most widely used plastic welding methods. Hot plate welding was used for pipelines and appliances as well as injection moldings. Numerous national and international associations for welding have specifications and guidelines for hot plate welding, including the Deutscher Verband fuer Schweissen (DVS) in Germany, the American Welding Society (AWS) in the United States, and the Comité Européen de Normalisation (CEN) in Europe.

Conventional hot plate welding
The hot plate welding process can be divided into four phases: matching, heating, change-over, and welding/forging.

The matching phase serves to match the geometry of the weld surfaces to the theoretical welding plane. The weld surfaces are heated through conduction by physical contact with the hot plate. The hot plate temperature range is 30 to 100 °C above the melting temperature of the material, and a constant pressure between 0.2 and 0.5 MPa is applied against the hot plate. This causes the weld surfaces to conform to the hot plate, which has the desired weld geometry. This also removes surface irregularities that would increase thermal contact resistance. After the parts are in full contact with the hot plate, the heating phase starts and pressure is reduced to a minimum.

During the heating phase, the weld region is heated conductively until melted, without substantial displacement of the material. Pressure is maintained either at a minimum to keep the parts and the hot plate in contact or at zero with a preset displacement. The melt surface reaches approximately 20 °C below the temperature of the hot plate. The viscosity of the melted material can be controlled through the temperature of the hot plate and the heating time. The surface of hot plate is often coated with PTFE to stop the molten plastic from sticking, which limits the hot plate temperature to 270 °C. The temperature of the parts during this phase can be modeled by assuming a constant temperature boundary condition and using the one-dimensional heat equation:


 * $$\theta(x,t) = \theta_i + (\theta_s - \theta_i) \cdot \operatorname{erfc} \left(\frac{x}{2\sqrt{\kappa t}}\right)$$

where θ is the temperature, x is the position, t is the time, θi is the initial temperature, θs is the constant surface temperature, κ is the thermal diffusivity, and erfc is the complementary error function. This model is valid for most cases, since the thermal contact resistance is low and the thermal mass of the hot tool is large compared to the plastic parts. For more precise predictions of the heat flow, the thermal contact resistance and the temperature dependence of the thermal properties of the plastic also need to be considered.

After sufficient heating time, the change-over phase begins. During this phase, the parts are retracted from the hot plate, the plate is quickly moved away, and the parts are brought together. The change-over should be as short as possible, because the melted region cools off during this time.

The welding/forging phase begins when the two molten surfaces are pressed together. This creates intermolecular diffusion of the plastic molecules according to reptation theory. Weld strength is provided by entanglement of the diffused plastic molecules. The necessary welding pressure depends on the melt viscosity and wall thickness of the parts and usually ranges between 0.025 and 0.05 MPa. This pressure is maintained while the melted material cools and resolidifies. During this, some plasticized material in the weld zone is squeezed out, forming flash. Mechanical stops may be used to limit the amount of squeezed out material in order to prevent a cold weld.

Variants
Common variants of conventional hot plate welding include high-temperature and non-contact versions. Both of these variants help with the problem of material sticking to the hot plate between weld cycles; the stuck material can degrade and transfer to subsequent welds, resulting in poor quality and aesthetically unappealing welds.

With high-temperature hot plate welding, an uncoated hot plate is heated to between 300 and 400 °C, as the PTFE coating degrades at high temperatures. The high temperature decreases the viscosity of the melt, so it can peel off from the hot plate when removing the parts. This can be accompanied during the change-over phase by rapid movement of the parts from the hot plate; this prevents stringing of the melted plastic due to its viscoelastic properties. Any residual material on the hot plate's surface is usually either oxidized away or mechanically removed. With some thermoplastics, the residual material cannot be easily removed and accumulates over time. The hot plates may need to be removed and cleaned between cycles. With the higher temperatures, the matching and heating phases are shortened from those of conventional hot plate welding. However, reduced weld strength from thermal degradation of the plastic can still occur, though most of the degraded material is forced out by the flow of melted material. High-temperature hot plate welding is known to perform well for:
 * PP and PP copolymers
 * ABS and PMMA

With non-contact hot plate welding, the weld surfaces are melted without physical contact with the hot plate through convection and radiation heating. The hot plate temperature is between 400 and 550 °C, and the weld surfaces are placed about 1 to 3 millimeters from the hot plate. Heat input needs to be controlled to prevent thermal degradation while plasticizing the material. This variant has no matching phase, so part fit must be good prior to welding, with part deviation not exceeding 0.2 millimeters. In practice, non-contact hot plate welding is only used for small parts whose dimensions do not exceed 100 by 100 millimeters. An additional consideration is the stack effect when the hot plate is oriented vertically, which can cause uneven heating of the weld surfaces.

Another variant is hot wedge or hot shoe welding for joining thin sheets with lap seams. A heated wedge travels between the two sheets and melts the weld surfaces while wedge rollers apply light pressure to force intimate contact; drive rollers apply pressure at the tip of the wedge where the sheets converge to form a continuous seam. Hot wedge welding can produce either single or dual seam joints. For dual seam joints, a split wedge that is unheated in the middle is used. This leaves an unwelded air pocket between the seams that can be pressurized to nondestructively test the joint integrity. With hot wedge welding, the speed of travel is an added parameter as the wedge unit is self-propelled by the rollers. The typical temperature range when welding high-density polyethylene (HDPE) is 220 to 400 °C; the travel speed is typically 0.7 to 4 meters per second.

Parameters
Parameters used in hot plate welding are the hot plate temperature, the pressure (or displacement) during matching, the pressure during heating, the pressure and displacement during the weld phase, and the times for matching, heating, change-over and cooling. These parameters have an interdependent effect on the weld quality and cannot be set individually.

The hot plate temperature is taken at the surface of the plate. It is set based on the hot plate welding variant along with the properties of the material, including melting temperature, melt viscosity, and thermal degradation limits. Conventional hot plate welding uses temperatures 30 to 100 °C above the melting temperature. The high-temperature variant uses temperatures above the material's degradation temperature, about 100 to 200 °C above the melting point. The non-contact variant uses temperatures 300 to 400 °C above the melting point. With non-contact welding, the radiation heating depends not only on the temperature but also on the emissivity of the hot plate material.

The pressure during the matching phase removes warpage of the weld surfaces to ensure full contact with the hot plate without causing the parts to deform. During the heating phase, a minimum pressure is maintained to keep the parts in contact with the hot plate, as a larger pressure would squeeze out material. The welding pressure brings the molten weld surfaces into intimate contact and squeezes out entrapped air. Too high a pressure would squeeze out most of the hot material from the joint, leaving cooler material to form a cold weld. Too low a pressure limits intermolecular diffusion and produces a weak weld. A mechanical stop may be used in the welding phase to limit the amount of material squeeze out by varying the welding pressure.

The matching and heating times control the amount of heat input during those phases. The matching time is set so that surface irregularities are melted and removed. The heating time determines the melt layer thickness. Too thick a melt results in excess flash and unfavorable molecular orientation at the joint interface. Too thin a melt produces a brittle weld. The change-over time determines the temperature of the melted material as welding begins and, therefore, should be as short as possible to minimize surface cooling. Typical change-over times are around 2 to 3 seconds, even for large parts. Cooling time refers to the time until the joined parts have solidified (when the molten material has cooled below its melting temperature) and can be removed from the machine. The welded part should not be stressed until it has further cooled until room temperature.

Material weldability
Hot plate welding can be used for joining all thermoplastics and thermoplastic elastomers whose melting temperature range lies below their decomposition temperature. Since only the plastic itself can be joined, additives, used to improve material properties or reduce cost, can reduce weldability. Additives can also reduce weld strength by acting as stress concentrators. Examples of additives include stabilizers, lubricants, processing aids, coloring agents, reinforcing materials (talcum, glass fibers, carbon fibers, etc.).

The water content of the plastic also affects weldability. This affects thermoplastics that absorb water from the surrounding air, mainly amorphous thermoplastics. High water content can lead to the formation of bubbles during heating and joining, reducing weld strength. Therefore, parts should be welded shortly after injection molding, stored in a dry environment, or welded with adjusted parameters.

Hot plate welding can be used to join some combinations of dissimilar thermoplastics. Typically, semi-crystalline plastics are only compatible with semi-crystalline plastics, and amorphous plastics are only compatible with amorphous plastics. If the plastics have the same melting point and melt viscosity, conventional or high-temperature hot plate welding can be used. With different melting points or different viscosities, dual hot plates should be used, with each hot plate set to a different temperature. Common thermoplastic combinations include:
 * ABS – PMMA
 * ABS – PC
 * ABS – SAN
 * PMMA – PC + ABS
 * PC – PC + ABS

Applications
Hot plate welding is used for joining parts ranging from a few centimeters up to 1.6 meters. It is also used for making continuous welds in lining membranes. Its usage can be divided into two main categories, namely production applications and pipe welding. These differ in their equipment and joint designs.

Production applications
One major industry using hot plate welding is the automotive sector. Tail light housings made of ABS are joined with lenses made of either PMMA or PC using a modified butt joint. ABS and PMMA have similar melting temperatures and can be welded using a single hot plate, while ABS and PC requires dual hot plates due to PC's higher melting temperature. Vacuum suction cups are used to move the parts to prevent scuffing. Both conventional and high-temperature variants are used. A typical cycle time is 60 seconds with a hot plate temperature of 370 °C.

Fuel tanks made of blow-molded HDPE need as many as 34 parts welded to it, including clips, filler necks, vent lines and brackets. The parts are welded individually using groove butt joints. Each component needs a different matching time, and cycle times are less than a minute per component.

The cases and lids of automotive batteries are made of thin PP copolymers, which have low melt viscosity. High-temperature hot plate welding is used on butt joints with flash covers. A typical machine can weld two batteries in a time of less than 30 seconds.

Other automotive components welded by hot plate are carburetor floats, coolant and washer fluid reservoirs, and ventilation ducts. Non-automotive items include dishwasher spray arms, laundry detergent boxes, steam iron reservoirs, HDPE barrels, PP transport pallets, medical needle disposal boxes, and PVC window frames.

Pipe welding
Hot plate welding, referred to as fusion welding in many industries, is commonly used to join plastic pipes. These pipes, as opposed to steel ones, are less likely to rupture during an earthquake. Pipe welding uses special joint configurations, namely butt, socket and saddle/sidewall, each with its own welding procedures.

Butt fusion welding has similar process phases as conventional hot plate welding. Before welding, the pipe ends are faced and the profiles are rounded and aligned with each other. The remaining phases proceed as normal, though sometimes the matching phase can be skipped. When welding dissimilar plastics, in lieu of dual hot plates, the pipe with the lower melt flow index can be heated earlier than the other, such that both pipe ends have the same melt viscosity at the end of the heating phase. After cooling, the flash bead is sometimes removed to leave smooth surfaces on the interior and exterior. Problems with the weld can be determined by inspecting this bead.

Socket fusion welding uses male and female heating tools attached to a hot plate to heat the exterior of the pipe and the interior of the socket simultaneously. This is typically used for pipes ranging from 40 to 125 millimeters. With this joint, the welding pressure is supplied by the interference fit of the pipe and socket, so these parts as well as the heating tools need to be within tolerance.

Saddle/sidewall fusion welding is used for joining saddle fittings onto the sidewall of a pipe to create branches. The exterior of the pipe and the matching surface of the saddle fitting are heated using concave and convex heating tools. The saddle fusion machine applies welding force through the centerline of the pipe. Prior to welding, the exterior of the pipe needs to be cleaned of all contaminants, because the melt layer of the pipe is not displaced from the joint.